Supporting hydrogen saturated 0.1 M Na2SO4 electrolyte by cyclic voltammetry curves, with using...
Embed Size (px)
Transcript of Supporting hydrogen saturated 0.1 M Na2SO4 electrolyte by cyclic voltammetry curves, with using...
Ambient Electrocatalytic Nitrogen Reduction on
MoO2/Graphene Hybrid: Experimental and DFT studies Jing Wang1#, Ya-ping Liu1#, Hu Zhang2, Da-jian Huang1, Ke Chu 1*
1 School of Materials Science and Engineering, Lanzhou Jiaotong University, Lanzhou 730070, China 2 School of Materials Science and Engineering, University of Science and Technology Beijing, Beijing, 100083, China *Corresponding author. E-mail address: firstname.lastname@example.org (K. Chu) # These authors contributed equally to this work.
Electronic Supplementary Material (ESI) for Catalysis Science & Technology. This journal is © The Royal Society of Chemistry 2019
Synthesis of MoO2/RGO
All the chemicals were used as received without further purification. The
MoO2/RGO was synthesized by a microwave-assisted hydrothermal approach based
on a reported method with a slight modification. Briefly, 50 ml of homogeneous
GO suspension (1 mg mL-1) was fabricated by dispersion of GO powder in distilled
water under ultrasonication for 1 h. Then, 0.4 g of ammonium molybdate tetrahydrate
and 0.04 g of ascorbic acid were sequentially added into GO suspension under
vigorous stirring for 10 min. After that, the mixture was sealed and treated by a
household microwave oven (2450 MHz) for 10 min. After cooling to room
temperature, the precipitates were collected and washed several times with distilled
water and then dried at 60°C for 12 h. Finally, the obtained powder was annealed at
400 °C for 2 h under Ar atmosphere. For comparison, the MoO2 NPs and RGO alone
were synthesized by the same procedure without addition of GO and ammonium
molybdate tetrahydrate, respectively.
Electrochemical NRR measurements
Electrochemical measurements were performed on a CHI-660E electrochemical
workstation using a standard three-electrode system, including Ag/AgCl electrode as
the reference electrode, graphite rod as the counter electrode and catalyst loaded on
carbon cloth (CC) as the working electrode. The working electrode was prepared by
loading 0.2 mg cm-2 of catalyst onto the CC (1 × 1 cm2). All potentials were
referenced to a reversible hydrogen electrode (RHE) by ERHE = EAg/AgCl + 0.197 +
0.059 × pH. The RHE calibration was experimentally conducted in the high-purity
hydrogen saturated 0.1 M Na2SO4 electrolyte by cyclic voltammetry curves, with using
graphite rod and Pt wire were used as the counter and working electrodes, respectively
(Fig. S1). Prior to electrolysis, the cathodic compartment was purged with Ar for 30
min. During the electrolysis, N2 gas (99.999% purity) was continuously fed into the
cathodic compartment at a flow rate of 10 mL min−1, and the electrolyte in the
cathodic compartment was subjected to magnetic stirring at a rate of 300 rpm
throughout the measurement. After electrolysis, the NH3 yield and FE were
determined by an indophenol blue method, and the possible N2H4 was determined
by a method of Watt and Chrisp.
Determination of NH3
The concentration of produced NH3 in 0.1 M Na2SO4 was quantitatively
determined by an indophenol blue method. Typically, 4 mL of electrolyte was
removed from the electrochemical reaction vessel. Then 50 μL of solution containing
NaOH (0.75 M) and NaClO (ρCl = ~4), 500 μL of solution containing 0.32 M NaOH,
0.4 M C7H6O3, and 50 μL of C5FeN6Na2O solution (1 wt%) were sequentially added
into the electrolyte. After standing for 2 h, the UV-Vis absorption spectrum was
measured and the concentration-absorbance curves were calibrated by the standard
NH4Cl solution with a serious of concentrations (Fig. S2a).
Determination of N2H4
The N2H4 concentration was quantitatively determined by a method of Watt and
Chrisp[3, 4]. Typically, 5 mL of electrolyte was removed from the electrochemical
reaction vessel. The 330 mL of color reagent containing 300 mL of ethyl alcohol, 5.99
g of C9H11NO and 30 mL of HCl were prepared, and 5 mL of color reagent was added
into the electrolyte. After stirring for 10 min, the UV-Vis absorption spectrum was
measured and the concentration-absorbance curves were calibrated by the standard
N2H4 solution with a serious of concentrations (Fig. S3a).
Calculations of NH3 yield and Faradaic efficiency
NH3 yield was calculated by the following equation:
(1)3cat. NH-1 1
NH yield ( g h mg ) =
c V t m
Faradaic efficiency was calculated by the following equation:
Faradaic efficiency (%) = 100% 17
F c V Q
where cNH3 is the measured NH3 concentration, V is the volume of the electrolyte, t is
the reduction time and m is the mass loading of catalyst on carbon paper. F is the
Faraday constant, Q is the quantity of applied electricity.
Scanning electron microscopy (SEM) was performed on a JSM-6701
microscope. Transmission electron microscopy (TEM) and high-resolution
transmission electron microscopy (HRTEM) were carried out on a Tecnai G2 F20
microscope. X-ray diffraction (XRD) pattern was recorded on a Shimadzu 7000LX
diffractometer. X-ray photoelectron spectroscopy (XPS) analysis was conducted on a
PHI 5702 spectrometer. Temperature-programmed desorption (TPD) profiles were
recorded on a Chem-BET 3000 (Quantachrome) apparatus. 1H (NMR) spectra were
collected on a 500 MHz Bruker superconducting-magnet NMR spectrometer.
DFT calculations were conducted using the CASTEP (Cambridge Serial Total
Energy Package) package. The Perdew-Burke-Ernzerhof (PBE) functional within the
framework of generalized gradient approximation (GGA) was applied to describe the
electron-electron interactions. The van der Waals forces were considered based on a
DFT-D3 correction method. For structural optimization, the Brillouin zone was
sampled by 3×3×1 k-points for plane-wave basis, together with a energy cutoff of 750
eV. The convergence criterions were set to 0.01 eV/Å and 10-5 eV for Hellmann-
Feymann force and total energy, respectively.
The formation Gibbs free energy (ΔG) of the NRR intermediates is calculated as
(3)U=G E ZPE T S G
where ΔE is the adsorption energy, ΔZPE is the zero point energy difference and TΔS
is the entropy difference between the gas phase and adsorbed state. ΔGU = -neU,
where n is the number of transferred charge and U is the electrode potential.
The adsorption energy (ΔE) was calculated by the following equation
(4)ads/s lab ads slab = E E E E
where Eads/slab, Eads and Eslab are the total energies for adsorbed species on slab,
adsorbed species and isolated slab, respectively.
Fig. S1. The RHE calibration in 0.1 M Na2SO4 electrolyte.
The RHE calibration was carried out in the high-purity hydrogen saturated 0.1 M
Na2SO4 electrolyte. The graphite rod and Pt wire were used as the counter and working
electrodes, respectively. The cyclic voltammetry curves were performed at 1 mV s-1 scan
rate. The RHE calibration potential for the hydrogen oxidation/evolution reactions is the
average value of the two potentials at which the current crosses zero. Accordingly, it is
shown in Fig. S1 that the E(RHE) is larger than E(Ag/AgCl) by 0.565 V, in good
accordance with the value of 0.569 V calculated by the Nernst equation: ERHE = EAg/AgCl
+ 0.197 + 0.059 × pH (6.3).
Fig. S2. XPS C1s spectra of MoO2/RGO
Working electrode Counter
Membrance Cathode Anode
Fig. S3. Photograph of H-type electrochemical setup
Fig. S4. (a) UV-Vis absorption spectra of indophenol assays with NH4Cl in 0.1 M Na2SO4 after incubated for 2 h at ambient conditions. (b) Calibration curve used for calculation of NH3 concentrations.
Fig. S5. (a) UV-Vis absorption spectra of N2H4 assays after incubated for 20 min at ambient conditions. (b) Calibration curve used for calculation of N2H4 concentrations.
Fig. S6. UV-Vis spectra of the electrolytes (stained with the chemical indicator based on the method of Watt and Chrisp) after 2 h electrocatalysis on MoO2/RGO at various potentials, and corresponding N2H4 concentrations in the electrolytes.
Fig. S7. UV-Vis absorption spectra of the electrolytes (stained with indophenol indicator) after standing for 2 h in open air of lab, or in electrochemical cell, or by continuously supplying N2, as well continuously supplying Ar.
As reported in the literature, the NH3 is ubiquitous in the laboratory
environment and is a common contaminant in chemicals, especially gases, which may
cause an overestimation of NRR performance. Therefore, before NRR electrolysis,
the background NH3 concentration in the laboratory environment was firstly
conducted. As shown in Fig. S7, f